RELATIONSHIP OF PAVING ASPHALT TEMPERATURESUSCEPTIBILITY AS MEASURED BY PVN TO PAVING ASPHALT
SPECIFICATIONS, ASPHALT PAVING MIXTURE DESIGN ANDASPHALT PAVEMENT PERFORMANCE
NORMAN W. McLEOD1
A s a measure of paving asphalt temperature susceptibility, PVN is an abbrevi-ation for pen-vis number, which in turn is a shortened version of penetrationat 25 C (77 F)-viscosity at 135 C (275 F) number, since as will be explainedlater, PVN is evaluated from the penetration at 25 C (77 F) and correspondingviscosity at 135 C (275 F) of paving asphalts from asphalt based wax freecrude oils, insofar as any asphalt is entirely free from wax.
In 1947, light waxy crude oils that provided asphalt of high temperaturesusceptibility were discovered in Western Canada in large volume. Shortly af-terward, the Canadian Federal Government decreed that all petroleum productsmarketed west of the Ontario-Quebec border had to be made from these crudeoils.
Up to that time most of the asphalt used in Ontario came from Venezualancrude oils that were refined in Montreal in the Province of Quebec. They hadlow temperature susceptibility and a high viscosity at 135 C (275 F) (Group Ain Figure 14). Paving mixtures made with these asphalts were so stable that therollers could be operated right up to the spreader. On the other hand, pavingasphalts from these Western Canadian light waxy crude oils were of high tem-perature susceptibility and had very low viscosity at 135 C (275 F) (Group Cin Figure 14). Paving mixture immediately behind the spreader lacked the sta-bility to which contractors had become accustomed. Rolling had to be delayedto allow the paving mixtures to cool and develop sufficient stability to supportthe weight of the roller. As one Materials Engineer said facetiously, the rollerman operated the spreader in the morning and then got on the roller to roll inthe afternoon what he had spread in the morning.
The contractor complaints over delayed rolling were so serious that in 1960the Ontario Department of Highways constructed three six-mile Test Roadsabout 40 miles apart on existing highways in South Western Ontario, Figure 1.In each 6-mile Test Road there were three 2-mile pavement test sections. Adifferent paving asphalt was used in each of the three 2-mile test sections,2-miles were paved with 85/100 penetration asphalt of low temperature suscep-tibility (Group A), 2-miles were paved with 85/100 penetration of approxi-mately medium temperature susceptibility (Group B), while 85/100 penetrationasphalt of high temperature susceptibility (Group C), was used for the other 2-mile pavement section. The same three asphalts were replicated in the threeTest Roads. The results from these Test Roads will be referred to later.
Vice President and Asphalt Consultant McAsphalt Engineering Services Toronto. Ontario, Canada
SUSCEPTIBILITY MEASURED BY PVN
Figures 1: Locations of Four Ontario Test Roads.
Two or three years later, without waiting for results from its test roads, theOntario Department of Highways adopted a paving asphalt specification requir-ing that 85/100 penetration asphalt must have a minimum viscosity of 140 se-conds Saybolt Furol at 135 C (275 F), later changed to 280 centistokes at 135C (275 F). For the 150/200 penetration grade, the minimum viscosity at 135 C(275 F) was 200 centistokes. They rejected all asphalts of high temperaturesusceptibility and about half of those of medium temperature susceptibility.
Ontarios use of asphalts of three different temperature susceptibilities in itsthree Test Roads, and its adoption of minimum viscosities at 135 C (275 F) forits new specification for paving asphalts, led the writer (2,3,4 and 5) to won-der if temperature susceptibility for paving asphalts could be based on penetra-tion at 25 C (77 F) and viscosity in centistokes at 135 C (275 F). This paperwill attempt to show that PVN is the most useful measure of paving asphalttemperature susceptibility that has been proposed so far.
Since the pen-vis number (PVN) concept for expressing paving asphalt tem-perature susceptibility was originated by the writer about twenty years ago, ithas been slowly developed from isolated bits and pieces of information, someof them my own, but some from the publication of others. In many respects, ithas been like putting a jig-saw puzzle together, except that with a jig-saw puz-zle, from the beginning, one has a picture of the final grouping of pieces tofollow as a guide. When working with PVN, I have not had this picture of the
final assemblage to follow. Only within the past few months have I been ableto fit all the isolated bits of information together into a well organized whole,which is the subject of this paper.
As I, and I believe many others see it, the major asphalt paving problemstoday are centered very largely around the following six headings:
(A) A more useful paving asphalt specification.(B) Avoidance of low temperature transverse pavement cracking in winter.(C) Providing adequate pavement stability for summer traffic.(D) Elimination of pavement rutting.(E) Developing a much more rational method for pavement recycling.(F) Providing surface treatments with superior service performance.
In addition, the paper will show how each of the above six objectives canbe further improved by the incorporation of small percentages of suitable poly-mers into the paving asphalt.
The paper shows that when everything else is equal, aggregate etc., a majorpart of the solution for each of these six items involves providing asphalts withhigher viscosity at 135 C (275 F) for any given penetration at 25 C (77 F).That is, the paving asphalt must often have a lower temperature susceptibility.This is one of the basic purposes of pen-vis number (PVN), which as has beenstated, is evaluated from the penetration of a paving asphalt at 25 C (77 F) andthe corresponding viscosity at 135 C (275 F). In terms of their PVN values,Figure 14, which normally range from 0.0 to -1.5, all paving asphalts can beseparated into one or the other of three groups, Group A, low temperature sus-ceptibility (PVN from 0.0 to -0.5), Group B, medium temperature susceptibil-ity, (PVN from -0.5 to -l.0), and Group C, high temperature susceptibility,(PVN from -1.0 to -1.5). Therefore, particularly for pavements for highertraffic volumes, PVN points the way toward asphalts of lower temperature sus-ceptibility to solve the six problems previously referred to.
Figure 2 illustrates that two-thirds of the U.S.A. North of the Mason-DixonLine has a frost penetration in winter ranging from 18 in. in the south to 72 in.in Northern Minnesota. Still greater depths of frost penetration occur inCanada and Alaska. Because of the repeated contraction and expansion stressescaused by changing temperatures in winter, this can result in severe low tem-perature transverse pavement cracking, in which no engineer could take anypride, in expensive maintenance for crack filling and other repairs, and in theunseen costs of shortened pavement service lives. Unstable pavements undersummer traffic are subject to rutting and to other forms of pavement distortionbecause of the lack of adequate pavement stability. Pavement recycling is in-creasing, but current methods of design seem to be ill-considered and inade-quate. They appear to be geared for short range success but at the expense ofthe same pavement deterioration in the long run that led to their recycling inthe first place. A more rational method with much improved long range servicelife is proposed. More serviceable surface treatments can also be constructed.
PAVING ASPHALT TEMPERATURE SUSCEPTIBILITY AND PVN
The temperature susceptibility of a paving asphalt is the change in the con-sistency (viscosity or penetration of the asphalt) for a given change in its tem-perature. As shown by Figure 3, taken from ASTM D 2493, a straight linegraph results when the log log viscosity of an asphalt is plotted versus the logof its absolute temperature. The slope of this line provides the temperature sus-ceptibility of the asphalt.
Figure 4 is taken from a small portion of Figure 3, and illustrates the tem-perature susceptibility of three asphalts, all of which have the same consistencyat 25 C (77 F). Because it has the steepest slope, Asphalt 3 in Figure 4 is saidto have high temperature susceptibility, since for the three asphalts illustratedin Figure 4, its consistency changes the most for a given change in tempera-ture. Since its slope changes the least for a given change in temperature, As-phalt 1 in Figure 4 is said to have low temperature susceptibility. Because theslope of Asphalt 2 is in-between the slopes of the other two asphalts in Figure4, Asphalt 2 is said to have intermediate or medium temperature susceptibility.
Figure 5 illustrates the five principal methods that have been proposed asmeasures of paving asphalt temperature susceptibility. The first, penetration ra-tio, is based upon penetrations at 4 C and 25 C (39 F and 77 F). It has had lo-cal application but does not appear to have been adopted on a national scale.
The second, viscosity temperature susceptibility, (VTS), has been promotedby The Asphalt Institute as a criterion for paving asphalt temperature suscepti-bility. As shown on Figure 5, VTS is based on the difference in log log vis-cosity at each of two temperatures, usually 135 C (275 F) and 60 C (140 F),divided by the difference in the logs of the same two absolute temperatures.This equation reduces temperature susceptibility to a very small number, sincefor example, the value of log log 1000 is only 0.4771 and for 500 is only0.4312, with the difference between them being only 0.0459. With such smallnumbers, the supporters of VTS, who refuse to admit that temperature suscep-tibility is an important property of paving asphalts, can argue that paving as-phalt temperature susceptibility either does not exist, or that it is not signi-ficant, or that it is merely the result of experimental error. This is illustratedby the following data for two asphalts that were obtained by The Asphalt In-stitute:
Penetration at 25 C (77 F) 119 103Viscosity at 60 C (140 F) (poises) 808 2222Viscosity at 135 C (275 F) (Cst) 223 540VTS 3.67 3.34Difference in VTS = 3.67 - 3.34 = 0.33PVN -0.94 +0.28Difference in PVN = +0.28 -(0.94) = 1.22
Note: the PVN values have been added for comparison.
In his AAPT paper of 1970, Lefebvre (4) provided Figure 6, which showsthe ratio between viscosity in poises at 60 C (140 F) and viscosity in centi-stokes at 135 C (275 F). Figure 6 indicates that this ratio varies with both
SUSCEPTIBILITY MEASURED BY PVN 419
penetration at 25 C (77 F) and with PVN (although it was not called PVN atthat time), and that its value ranges from about one to eight.
As a basis for paving asphalt specifications, the asphalt suppliers encouragedboth ASTM and AASHTO to change the method for grading paving asphaltsfrom penetration at 25 C (77 F) to grading them by viscosity in poises at 60 C(140 F), with the resulting five grades, AC 2.5, AC 5, AC 20, AC 20, and AC40, Figure 7, to which a sixth grade AC 30 was added later.
Figure 8 shows how these five viscosity grades at 60 C (140 F) appearwhen they are plotted on a chart in terms of PVN values. Both Figures 6 and 8demonstrate that the relationship between viscosity in poises at 60 C (140 F)and viscosity in centistokes at 135 C (275 F) is not simple.
Pfeiffer and Van Doormaal of the Royal Dutch Shell Laboratories at Am-sterdam, Holland, in a paper published in 1936 (6), adopted a very differentapproach for the measurement of paving asphalt temperature susceptibility,which they named penetration index, or PI. As an axis for reference theybased their zero PI on a Mexican asphalt of 200 penetration at 25 C (77 F) thatwas derived from a wax free asphalt based crude oil. To measure the temper-ature susceptibilities of various paving asphalts, they prepared a nomograph,Figure 9, for which the penetration at 25 C (77 F) and the ring and ball soften-ing point of a paving asphalt were required, as indicated by Equation 3 on Fig-ure 5. To use this nomograph, a straight line was drawn from the pointrepresenting the penetration test value on the ordinate on the right, which listsvalues for the penetration test at whatever temperature in C it was measured,usually 25 C (77 F), to a corresponding point on the ordinate on the left,which marks the difference in temperature in C between the ring and ballsoftening point and the temperature at which the penetration test was made.The value indicated by the point where this line intersects the oblique linerepresenting penetration index, or PI, indicates the PI of the paving asphalt.
As shown by Equation 3 in Figure 5, values for the penetration of a pavingasphalt at 25 C (77 F) and for its ring and ball softening point temperature arerequired for Pfeiffers and Van Doormaals temperature susceptibility measure-ment in terms of PI. However, because of small quantities of wax retained inpaving asphalts made from Western Canadas light waxy crude oils, the soften-ing point temperatures were much too high. They exceeded the softening pointtemperatures of paving asphalts otherwise the same but free from wax. Thismade Pfeiffers and Van Doormaals equation useless for expressing the tem-perature susceptibilities of paving asphalts from these waxy crude oils.
Heukelom (7) attempted to overcome the effect of wax in these pavingasphalts by making penetration tests at 4 C, 10 C and 25 C, and extending theleast squares line through these values to obtain the temperature correspondingto a penetration of 800, since for many asphalts this corresponded approxi-mately to the ring and ball softening point temperature. Heukelom substitutedthis temperature for the ring and ball softening point temperature in Pfeifferand Van Doormaals equation to obtain a corrected value for PI, or the PIcould alternatively be taken from Shells Bitumen Test Data Chart (7). How-ever, as will be shown shortly, Heukelom appears to have over-corrected forwax content. Consequently, for asphalts from these light waxy crude oils,
Figure 11: Illustrating Relationships between Penetration at 77F, Softening Point F(Ring and Ball), and Penetration Index (PI) Values of 0.0 and -1.5 for Paving AsphaltsManufactured by Steam or Vacuum Reduction.
asphalts from appropriate wax free asphalt based crude oils, matched Pfeifferand Van Doormaals PI of -1.5 for the same asphalts Figures 10, 11 and 12.
In the Appendix to my 1972 AAPT paper (S), I show a rough plot of vis-cosity SSF at 275 F (135 C) versus penetration at 77 F (25 C) for 10 asphaltswith a Pfeiffer and Van Doormaal PI of 0.0, Figure 10, which also shows asimilar plot for Pfeiffer and Van Doormaal penetration index, PI of -1.5. Thelines representing PI = 0.0 and PI = -1.5 in Figure 10 were drawn as bestlines through the data. The data illustrated in Figure 10 came from an internalreport...